temperature dependence of structural and ... physical review b 85, 035125 (2012) temperature...
Post on 16-Aug-2020
Embed Size (px)
PHYSICAL REVIEW B 85, 035125 (2012)
Temperature dependence of structural and electronic properties of the spin-liquid candidate κ-(BEDT-TTF)2Cu2(CN)3
Harald O. Jeschke,1 Mariano de Souza,2,* Roser Valentı́,1 Rudra Sekhar Manna,2 Michael Lang,2 and John A. Schlueter3 1Institut für Theoretische Physik, Goethe-Universität Frankfurt am Main, D-60438 Frankfurt am Main, Germany
2Physikalisches Institut, Goethe-Universität Frankfurt am Main, D-60438 Frankfurt am Main, Germany 3Materials Science Division, Argonne National Laboratory, Argonne, Illinois 60439, USA
(Received 21 November 2011; revised manuscript received 10 January 2012; published 27 January 2012)
We investigate the effect that the temperature dependence of the crystal structure of a two-dimensional organic charge-transfer salt has on the low-energy Hamiltonian representation of the electronic structure. For that, we determine the crystal structure of κ-(BEDT-TTF)2Cu2(CN)3 for a series of temperatures between T = 5 and 300 K by single crystal X-ray diffraction and analyze the evolution of the electronic structure with temperature by using density functional theory and tight binding methods. We find a considerable temperature dependence of the corresponding triangular lattice Hubbard Hamiltonian parameters. We conclude that even in the absence of a change of symmetry, the temperature dependence of quantities like frustration and interaction strength can be significant and should be taken into account.
DOI: 10.1103/PhysRevB.85.035125 PACS number(s): 61.05.cp, 61.66.Hq, 75.10.Jm, 71.15.Mb
The two-dimensional organic charge-transfer salts based on bis(ethylenedithio)tetrathiafulvalene (BEDT-TTF or even shorter ET) molecules in a κ-type lattice arrangement have been intensively studied over the past 30 years due to their complex interplay between electron correlation and the effects of low dimensionality and spin frustration.1 In particular, the discovery of spin-liquid behavior in κ-(BEDT- TTF)2Cu2(CN)3 (Ref. 2) has fascinated experimentalists and theorists alike. Issues of current interest concern the nature of the low-temperature spin-liquid realized in this material3–5
and the various anomalies observed upon approaching the spin-liquid state from high temperatures. These anomalies include drastic changes in the 1H-NMR relaxation rate around 200 to 150 K (Ref. 6), the thermopower at 150 K (Ref. 7), relaxor-type ferroelectricity around 60 K (Ref. 8), and a mysterious phase-transition anomaly at 6 K (Ref. 9). The latter feature, which manifests itself in anomalies in thermodynamic2,3 and transport4 quantities, is accompanied by pronounced lattice effects.9 Various scenarios have been suggested for the 6 K anomaly including a crossover from a thermally to a quantum disordered state,3 an instabil- ity of the quantum spin-liquid,3,10–16 or a distinct type of charge ordering.17 Theoretically, the spin-liquid properties have been investigated on the basis of the anisotropic triangular-lattice Hubbard Hamiltonian.12,18–21 The parame- ters t , t ′, and U of this Hamiltonian have been determined with semiempirical7 as well as first principles methods22,23
based on the experimental structure at room temperature. Missing in such investigations is, however, the consider- ation of a possible temperature dependence of the model parameters.
In this work, we find by a combination of single crystal X-ray diffraction at various temperatures and density func- tional theory calculations that even in the absence of structural phase transitions, the temperature dependence of the structural parameters is significant enough to influence the electronic behavior and the determination of the Hamiltonian model parameters in κ-(BEDT-TTF)2Cu2(CN)3. We suggest that this
has subtle effects on the degree of frustration and interaction strength.
In 1991, the crystal structure of κ-(BEDT-TTF)2Cu2(CN)3 was reported,24 and the unit cell parameters confirmed,25 on twinned crystals at room temperature. The crystal structure was redetermined in 1993, also on a twinned crystal at room temperature.26 The crystal structure of the very similar κ ′- (BEDT-TTF)2Cu2(CN)3 structure, which is reported to be an ambient pressure superconductor, was described in 1992.27,28
The crystal structure of the κ phase was subsequently redeter- mined in 1997,29 and the unit cell redetermined in 2001, both at room temperature.30 Already in 1991, the unit cell parameters were reported at 300 and 30 K, with a(30 K)/a(300 K) = 0.9964, b(30 K)/b(300 K) = 0.9932, c(30 K)/c(300 K) = 0.9900, and β(30 K)/β(300 K) = 1.0146 (Ref. 31). Our comparable con- traction values between 300 and 20 K are a(20 K)/a(300 K) = 0.9988, b(20 K)/b(300 K) = 0.9958, c(20 K)/c(300 K) = 0.9905, and β(20 K)/β(300 K) = 1.0148 and agree well with the previous results. In addition, we find evidence for an ordering of the ethylene groups in a staggered conformation between 200 and 150 K. Despite the current interest in this material as a spin-liquid candidate, no low-temperature structural determinations have yet been reported. Herein, we present a detailed characterization of the crystal structure as function of temperature determined on a single crystal with very high agreement factors.
II. SINGLE CRYSTAL X-ray DIFFRACTION
A black, platelike crystal of κ-(BEDT-TTF)2Cu2(CN)3 with dimensions 0.4 × 0.4 × 0.4 mm3 was placed onto the tip of a glass fiber and mounted on a Bruker APEX II three-circle diffractometer equipped with an APEX II detector. Temperature control in the 100–300 K region was provided by an Oxford Cryostream 700 Plus Cooler, while below 100 K it was provided by a Cryocool-LHE cryogenic system (Cryo Industries of America). The sample temperature below 100 K was confirmed by installing a Cernox thermometer (Lakeshore) in the immediate vicinity of the crystal and
035125-11098-0121/2012/85(3)/035125(7) ©2012 American Physical Society
HARALD O. JESCHKE et al. PHYSICAL REVIEW B 85, 035125 (2012)
FIG. 1. (Color online) Structure of κ-(BEDT-TTF)2Cu2(CN)3 at T = 5 K. Note that the disordered CN− group in the inversion center is only shown in one conformation.
stabilizing the temperature immediately prior to data collec- tion. In order to reduce adverse thermal effects, the thermome- ter wires (twisted manganin wires, 0.5-mm diameter, supplied by Lakeshore) were anchored on the surfaces of the cryostat exposed to the 4He stream. The data were collected using MoKα radiation (λ = 0.71073 Å) with a detector distance of 50 mm. Unit cell parameters were determined upon cooling in 10 K increments between 100 and 290 K, with a frame exposure time of 10 s. Full data sets for structural analysis were collected at temperatures of 5, 20, 100, 150, 200, 250,
and 300 K. The uncertainties in the temperature determination are typically ±0.2 K down to 100 K, while for the 20 and 5 K data points, an error bar of ±1 K has to be accepted. These data collections nominally covered over a hemisphere of reciprocal space by a combination of three sets of exposures. Data to a resolution of 0.68 Å were considered in the reduction. The raw intensity data were corrected for absorption [SADABS (Ref. 32)]. The structure was solved and refined using SHELXTL (Ref. 33). A direct-method solution was calculated, which pro- vided most of atomic positions from the electron-density map. Full-matrix–least-squares/difference-Fourier-cycles were per- formed, which located the remaining atoms. All nonhydrogen atoms were refined with anisotropic displacement parameters. The hydrogen atoms were placed in ideal positions and refined as riding atoms with relative isotropic displacement parameters.
As a representative example, in Fig. 1 we show the structure of κ-(BEDT-TTF)2Cu2(CN)3 at a temperature of T = 5 K. In the bc plane, the BEDT-TTF molecules form their typical κ-type arrangement. One of the cyanide (CN−) groups resides on an inversion center, thus requiring it to be disordered with a 50% carbon and 50% nitrogen distribution on these two atomic positions.24 Analysis of the low-temperature structural data (see Table I) indicates that overall, a, b, and c axes decrease with temperature, while the β angle increases monotonically upon cooling. We find that the orthogonal projection of the a axis, a⊥ = a sin β, has the greatest relative contraction with temperature. One ethylene group is disordered at room temperature with a staggered conformation 77% of the time. As the temperature is lowered, the ethylene group remains partially disordered down to a temperature of 200 K and is fully ordered in a staggered conformation at 150 K. The anion layer becomes slightly more buckled at low temperature: at room temperature, the Cu1 atom lies 0.050 Å out of the
TABLE I. Crystal data and structure refinement of κ-(BEDT-TTF)2Cu2(CN)3. Formula = C23H16Cu2N3S16, formula weight MW = 974.43, monoclinic, wavelength λ = 0.71073 Å, effective number of electrons in the crystal unit cell contributing to F(000) = 978, space group P 21/c, Z = 2. Residual factor for the reflections R1 =
∑ ||Fo| − |Fc||/∑ |Fo|, weighted residual factors wR2 = [∑w(F 2o − F 2c )2/∑w(F 2o )2] 12 , I > 2σ (I ), least-squares goodness-of-fit parameter GoF = [∑w(F 2o − F 2c )2/(Nd − Np)] 12 . Staggered (%) is the percentage of ethylene groups that are in the staggered conformation. Note that in eclipsed and staggered conformations, the two ethylene end groups have the same or opposite twist angle with respect to the plane of the molecule, respectively. dCu−NNC (Å) is the distance that the Cu(I) ion is out of the plane defined by the coordinated N, N, and C atoms. The